title: ÐÑÑÐ»ÐµÐ´Ð¾Ð²Ð°Ð½Ð¸Ðµ Ð¿ÑÐ¾ÑÐµÑÑÐ° Ð¿Ð¾Ð»ÑÑÐµÐ½Ð¸Ñ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ¸Ð¾Ð½Ð½ÑÑ Ð¼Ð°ÑÐµÑÐ¸Ð°Ð»Ð¾Ð² ÑÐ¸ÑÑÐµÐ¼Ñ Ð°Ð»ÑÐ¼Ð¸Ð½Ð¸Ð¹-ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½Ð¾Ðµ Ð²Ð¾Ð»Ð¾ÐºÐ½Ð¾
title: Ð²ÑÐ¿ÑÑÐºÐ½Ð°Ñ ÐºÐ²Ð°Ð»Ð¸ÑÐ¸ÐºÐ°ÑÐ¸Ð¾Ð½Ð½Ð°Ñ ÑÐ°Ð±Ð¾ÑÐ° Ð¼Ð°Ð³Ð¸ÑÑÑÐ°
titleType: Subtitle
title: Study of the process of obtaining composite materials of the aluminum-carbon system fiber
Creators: name: ÐÐ¼Ð°Ð½ÑÐ»Ð»Ð°, Ð¢ÐµÐ³Ñ
Publisher: name: Ð¡Ð°Ð½ÐºÑ-ÐÐµÑÐµÑÐ±ÑÑÐ³ÑÐºÐ¸Ð¹ Ð¿Ð¾Ð»Ð¸ÑÐµÑÐ½Ð¸ÑÐµÑÐºÐ¸Ð¹ ÑÐ½Ð¸Ð²ÐµÑÑÐ¸ÑÐµÑ ÐÐµÑÑÐ° ÐÐµÐ»Ð¸ÐºÐ¾Ð³Ð¾
Year: 2023
Subjects: Ð°Ð»ÑÐ¼Ð¾Ð¼Ð°ÑÑÐ¸ÑÐ½ÑÐ¹ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸Ñ
ÑÐ»ÐµÐºÑÑÐ¾Ñ Ð¸Ð¼Ð¸ÑÐµÑÐºÐ¾Ðµ Ð¾ÑÐ°Ð¶Ð´ÐµÐ½Ð¸Ðµ
ÑÐµÑÐ¼Ð¾Ð¼ÐµÑ Ð°Ð½Ð¸ÑÐµÑÐºÐ°Ñ Ð¾Ð±ÑÐ°Ð±Ð¾ÑÐºÐ°
Ð´Ð¸ÑÑÑÐ·Ð¸Ð¾Ð½Ð½ÑÐ¹ Ð¿ÑÐ¾ÑÐµÑÑ
aluminium matrix composite
electrochemical deposition
thermomechanical treatment
diffusion process

description: Ð¦ÐµÐ»ÑÑ Ð´Ð°Ð½Ð½Ð¾Ð¹ ÑÐ°Ð±Ð¾ÑÑ ÑÐ²Ð»ÑÐµÑÑÑ Ð¿Ð¾Ð²ÑÑÐµÐ½Ð¸Ðµ Ð°Ð´Ð³ÐµÐ·Ð¸Ð¾Ð½Ð½Ð¾Ð¹ Ð¿ÑÐ¾ÑÐ½Ð¾ÑÑÐ¸ ÑÐ»Ð¾Ð¸ÑÑÐ¾Ð³Ð¾ Ð°Ð»ÑÐ¼Ð¾Ð¼Ð°ÑÑÐ¸ÑÐ½Ð¾Ð³Ð¾ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ°, Ð°ÑÐ¼Ð¸ÑÐ¾Ð²Ð°Ð½Ð½Ð¾Ð³Ð¾ ÑÐ³Ð»ÐµÐ²Ð¾Ð»Ð¾ÐºÐ½Ð¾Ð¼ Ñ Ð½Ð¸ÐºÐµÐ»ÐµÐ²ÑÐ¼ Ð¸ ÑÐ¸Ð½ÐºÐ¾Ð²ÑÐ¼ Ð¿Ð¾ÐºÑÑÑÐ¸ÑÐ¼Ð¸. ÐÑÑÐ»ÐµÐ´Ð¾Ð²Ð°Ð½Ð¸Ñ, Ð¿ÑÐ¾Ð²ÐµÐ´ÐµÐ½Ð½ÑÐµ Ð² ÑÐ°Ð¼ÐºÐ°Ñ Ð´Ð°Ð½Ð½Ð¾Ð¹ ÑÐ°Ð±Ð¾ÑÑ, Ð±ÑÐ»Ð¸ ÑÐ²ÑÐ·Ð°Ð½Ñ Ñ ÑÐ»ÑÑÑÐµÐ½Ð¸ÐµÐ¼ Ð°Ð´Ð³ÐµÐ·Ð¸Ð¾Ð½Ð½Ð¾Ð¹ Ð¿ÑÐ¾ÑÐ½Ð¾ÑÑÐ¸ Ð¼Ð°ÑÑÐ¸ÑÐ½ÑÑ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ¾Ð² Ð°Ð»ÑÐ¼Ð¸Ð½Ð¸Ð¹-ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½Ð¾Ðµ Ð²Ð¾Ð»Ð¾ÐºÐ½Ð¾. ÐÐ° Ð²Ð¾Ð»Ð¾ÐºÐ½Ð° Ð½Ð°Ð½Ð¾ÑÐ¸Ð»Ð¸ Ð´Ð²Ð° Ð¼ÐµÑÐ°Ð»Ð»Ð¸ÑÐµÑÐºÐ¸Ñ Ð¿Ð¾ÐºÑÑÑÐ¸Ñ Ð¸Ð· Ð½Ð¸ÐºÐµÐ»Ñ Ð¸ ÑÐ¸Ð½ÐºÐ° Ð´Ð»Ñ Ð·Ð°ÑÐ¸ÑÑ Ð¾Ñ Ð¼ÐµÐ¶ÑÐ°Ð·Ð½Ð¾Ð¹ Ð´ÐµÐ³ÑÐ°Ð´Ð°ÑÐ¸Ð¸, ÐºÐ¾ÑÑÐ¾Ð·Ð¸Ð¸ Ð¼ÐµÐ¶Ð´Ñ ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½ÑÐ¼ Ð°ÑÐ¼Ð¸ÑÐ¾Ð²Ð°Ð½Ð¸ÐµÐ¼ Ð¸ Ð°Ð»ÑÐ¼Ð¸Ð½Ð¸ÐµÐ²Ð¾Ð¹ Ð¼Ð°ÑÑÐ¸ÑÐµÐ¹, Ð° ÑÐ°ÐºÐ¶Ðµ Ð´Ð»Ñ ÑÐ»ÑÑÑÐµÐ½Ð¸Ñ Ð¿ÑÐ¾ÑÐ½Ð¾ÑÑÐ½ÑÑ ÑÐ°ÑÐ°ÐºÑÐµÑÐ¸ÑÑÐ¸Ðº Ð¿Ð¾Ð»ÑÑÐµÐ½Ð½Ð¾Ð³Ð¾ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ¸Ð¾Ð½Ð½Ð¾Ð³Ð¾ Ð¼Ð°ÑÐµÑÐ¸Ð°Ð»Ð°. ÐÑ Ð½Ð°Ð½Ð¾ÑÐ¸Ð»Ð¸ Ñ Ð¿Ð¾Ð¼Ð¾ÑÑÑ Ð¾Ð±ÑÑÐ½Ð¾Ð³Ð¾ ÑÐ»ÐµÐºÑÑÐ¾ÑÐ¸Ð¼Ð¸ÑÐµÑÐºÐ¾Ð³Ð¾ Ð¾ÑÐ°Ð¶Ð´ÐµÐ½Ð¸Ñ Ñ ÑÐ°Ð·Ð½ÑÐ¼ Ð²ÑÐµÐ¼ÐµÐ½ÐµÐ¼ Ð¿ÑÐ¾Ð¿Ð¸ÑÐºÐ¸ Ð´Ð»Ñ ÐºÐ°Ð¶Ð´Ð¾Ð³Ð¾ Ð¼ÐµÑÐ°Ð»Ð»Ð¸ÑÐµÑÐºÐ¾Ð³Ð¾ Ð¿Ð¾ÐºÑÑÑÐ¸Ñ. ÐÑÐ¾ÑÐµÑÑ Ð¸Ð·Ð³Ð¾ÑÐ¾Ð²Ð»ÐµÐ½Ð¸Ñ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ° Ð¾ÑÑÑÐµÑÑÐ²Ð»ÑÐµÑÑÑ Ñ Ð¿ÑÐ¸Ð¼ÐµÐ½ÐµÐ½Ð¸ÐµÐ¼ ÑÐµÑÐ¼Ð¾Ð¼ÐµÑÐ°Ð½Ð¸ÑÐµÑÐºÐ¾Ð¹ Ð¾Ð±ÑÐ°Ð±Ð¾ÑÐºÐ¸ Ð´Ð°Ð²Ð»ÐµÐ½Ð¸ÐµÐ¼ Ð² Ð¿Ð¾Ð»ÑÐ¾ÑÑ ÑÐ¾Ð½Ð½Ñ, ÑÐ°Ðº ÐºÐ°Ðº Ð·Ð°Ð²ÐµÑÑÐ°ÑÑÐ¸Ð¼ Ð¿ÑÐ¾ÑÐµÑÑÐ¾Ð¼ Ð±ÑÐ»Ð° ÑÐµÑÐ¼Ð¾Ð¾Ð±ÑÐ°Ð±Ð¾ÑÐºÐ° Ð¿ÑÐ¸ 200Â°Ð¡ Ð² ÑÐµÑÐµÐ½Ð¸Ðµ 5 ÑÐ°ÑÐ¾Ð². ÐÐ¾Ð»ÑÑÐµÐ½Ð½ÑÐµ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÑ Ð±ÑÐ»Ð¸ ÑÐ¾ÑÐ¾ÑÐ¾ Ð¿ÑÐ¾Ð¿Ð¸ÑÐ°Ð½Ñ Ð¸ Ð±ÑÐ»Ð¸ Ð¸ÑÐ¿ÑÑÐ°Ð½Ñ Ð½Ð° ÑÐ°ÑÑÑÐ¶ÐµÐ½Ð¸Ðµ Ð´Ð»Ñ Ð¾Ð¿ÑÐµÐ´ÐµÐ»ÐµÐ½Ð¸Ñ Ð¸Ñ Ð¼ÐµÑÐ°Ð½Ð¸ÑÐµÑÐºÐ¸Ñ ÑÐ²Ð¾Ð¹ÑÑÐ². ÐÐ¾Ð²ÑÑÐµÐ½Ð¸Ðµ Ð¿ÑÐµÐ´ÐµÐ»Ð° Ð¿ÑÐ¾ÑÐ½Ð¾ÑÑÐ¸ Ð¿ÑÐ¸ ÑÐ°ÑÑÑÐ¶ÐµÐ½Ð¸Ð¸ ÑÐµÐ»ÑÐ½Ð¾Ð¼ÐµÑÐ°Ð»Ð»Ð¸ÑÐµÑÐºÐ¾Ð³Ð¾ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ° Ñ Ð°ÑÐ¼Ð¸ÑÐ¾Ð²Ð°Ð½Ð½Ð¾Ð¹ ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½ÑÐ¼ Ð²Ð¾Ð»Ð¾ÐºÐ½Ð¾Ð¼ Ð°Ð»ÑÐ¼Ð¸Ð½Ð¸ÐµÐ²Ð¾Ð¹ Ð¼Ð°ÑÑÐ¸ÑÐµÐ¹ Ð¸Ð·ÑÑÐ°Ð»Ð¾ÑÑ Ð¿ÑÐ¸Ð¼ÐµÑÐ½Ð¾ Ð´Ð»Ñ 131 Ð¸ 147 ÐÐÐ° (Ñ Ð½Ð¸ÐºÐµÐ»ÐµÐ²ÑÐ¼ Ð¿Ð¾ÐºÑÑÑÐ¸ÐµÐ¼) Ð¸ 151 ÐÐÐ° (Ñ ÑÐ¸Ð½ÐºÐ¾Ð²ÑÐ¼ Ð¿Ð¾ÐºÑÑÑÐ¸ÐµÐ¼). ÐÐ¾Ð»ÐµÐµ Ð²ÑÑÐ¾ÐºÐ°Ñ Ð¿ÑÐµÐ´ÐµÐ»ÑÐ½Ð°Ñ Ð¿ÑÐ¾ÑÐ½Ð¾ÑÑÑ Ð½Ð° ÑÐ°ÑÑÑÐ¶ÐµÐ½Ð¸Ðµ Ð°Ð»ÑÐ¼Ð¾Ð¼Ð°ÑÑÐ¸ÑÐ½ÑÑ ÐºÐ¾Ð¼Ð¿Ð¾Ð·Ð¸ÑÐ¾Ð², Ð°ÑÐ¼Ð¸ÑÐ¾Ð²Ð°Ð½Ð½ÑÑ Ð²Ð¾Ð»Ð¾ÐºÐ½Ð¾Ð¼ Ñ ÑÐ¸Ð½ÐºÐ¾Ð²ÑÐ¼ Ð¿Ð¾ÐºÑÑÑÐ¸ÐµÐ¼, Ð¾Ð±ÑÑÑÐ½ÑÐµÑÑÑ Ð»ÑÑÑÐµÐ¹ ÐºÐ¾Ð¼Ð¿Ð°ÐºÑÐ½Ð¾ÑÑÑÑ Ð¼Ð°ÑÑÐ¸ÑÑ Ð¸ Ð»ÑÑÑÐ¸Ð¼ ÑÑÐµÐ¿Ð»ÐµÐ½Ð¸ÐµÐ¼ Ð½Ð° Ð³ÑÐ°Ð½Ð¸ÑÐµ ÑÐ°Ð·Ð´ÐµÐ»Ð° Ð²Ð¾Ð»Ð¾ÐºÐ½Ð¾-Ð¼Ð°ÑÑÐ¸ÑÐ°, ÑÑÐ¾ ÑÐ¿Ð¾ÑÐ¾Ð±ÑÑÐ²ÑÐµÑ ÑÐ¿Ð¾ÑÐ¾Ð±Ð½Ð¾ÑÑÐ¸ Ð¿ÐµÑÐµÐ´Ð°Ð²Ð°ÑÑ Ð½Ð°Ð³ÑÑÐ·ÐºÑ Ð¾Ñ Ð°Ð»ÑÐ¼Ð¸Ð½Ð¸ÐµÐ²Ð¾Ð¹ Ð¼Ð°ÑÑÐ¸ÑÑ Ðº ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½Ð¾Ð¼Ñ Ð²Ð¾Ð»Ð¾ÐºÐ½Ñ Ð² ÑÐ¾ÑÑÐ¾ÑÐ½Ð¸Ð¸ Ð½Ð°Ð³ÑÑÐ·ÐºÐ¸, ÑÑÐ¾ Ð´Ð°ÐµÑ Ð¿Ð¾Ð»Ð½ÑÑ ÑÐ²Ð¾Ð±Ð¾Ð´Ñ Ð½ÐµÑÑÑÐ°Ñ ÑÐ¾Ð»Ñ ÑÐ³Ð»ÐµÑÐ¾Ð´Ð½Ð¾Ð³Ð¾ Ð²Ð¾Ð»Ð¾ÐºÐ½Ð°.
description: The purpose of this work is to increase the adhesive strength of a layered aluminum matrix composite reinforced with carbon fiber with nickel and zinc coatings. The research conducted in this study was concerned with the improvement of adhesion strength of aluminium-carbon fibre matrix composites. Two metallic coatings of nickle and zinc were applied to the fibers to protect against interfacial degradation, corrosion between carbon reinforcement and aluminium matrix, as well as improving the strength characteristics of the resulting composite material. They were applied using common electrochemical deposition with different infiltration time for each metal coatings. The fabrication process of composite is done by using termomechanical treatment with the pressure of one and half tonnes as heat treatment was being a final processat 200ËC for 5 hours. The resultant composites were well-infiltrated and were tested in tension to determine their mechanical properties. Increasing of ultimate tensile strength of the all metall-coated carbon fiber-reinforced aluminum matrix composite werestudied for about 131 and 147 MPa (nickel-coated)and 151 (zinc-coated). The better ultimate tensile steength for zinc-coated fiber-reinforced composites are attributed to better compactness of the matrix and better fiberâmatrix interface bonding, which favor the load transfer ability from aluminam matrix to carbon fiber under the loading state, giving full play to the bearing role of carbon fiber.